### D

### IPARTIMENTO DI

### I

### NGEGNERIA DELL

### ’I

### NFORMAZIONE

### Corso di Laurea Magistrale in Ingegneria delle

### Telecomunicazioni

Tesi di Laurea

*“ Design of *

*Thin Electromagnetic Radar Absorbers using Commercial *

*Lossy Materials*

* ” *

Relatori Candidato

Prof. Agostino MONORCHIO Francesco SCARANO

Prof. Raj MITTRA Ing. Filippo COSTA Ing. Simone GENOVESI

### Ai miei genitori,

### a mio fratello

### A chi ha creduto in me

### a chi mi ha dato forza,

### a chi ha avuto la pazienza

### di aspettare

Tutti sanno che una cosa è impossibile da realizzare, finché arriva uno sprovveduto che non lo sa e la inventa.

*Abstract *

**A**

**BSTRACT**

This work is focused on techniques for designing thin wideband radar absorbers. After the definition and the characterization of metamaterials, the use of lossy materials and frequency selective surfaces in multilayer stratified media is discussed and some of the most promising designs found proposed in the literature are analyzed. A non-conventional frequency selective surface shape, based on Hilbert and Peano space-filling curves, is proposed and integrated in a classic dual layer absorbing structure. Finally a practical method to design an optimized absorber for normal and oblique incidence using the materials from a database is proposed. The use of commercial lossy materials manufactured by Emerson & Cuming, Inc., is investigated.

*Acknowledgements *

**A**

**CKNOWLEDGEMENTS**

I would first like to thank Prof. Monorchio for giving me the opportunity to spend six months in the USA and then, back in Italy, to work in his laboratory under his supervision, where I learned a lot. I would also like to thank Dr. Mittra for the hospitality at University of Central Florida, giving me the opportunity to work with his research group. Thanks for the help when I arrived in Orlando and for all the advices he gave me during the weekly meetings. I would like to acknowledge Ing. Filippo Costa, available at any time for me, ready to answer my questions and clarify any doubt I had with infinite patience. I am gratefully indebted for his very valuable comments on this thesis. My gratitude goes to Marco, who helped me to organize my experience in the US and gave me important suggestions for my work. Special thanks to Alessio and Michele, who dedicated their time to help me with the editing of this thesis, their advises were so precious; to Ing. Genovesi, Davide, Andrea and all the other members of the laboratory who helped me when I had doubt or problems with the simulations.

Thanks to Daniele, Marco and Renee for making my American experience unforgettable, we shared a beautiful experience and we grew up a bit together. I would like also to acknowledge my family for being present at any time in my life. Finally, I must express my very profound gratitude to my parents and to my brother for providing me with unfailing support and continuous encouragement throughout my years of study. Thanks for the patience and for the possibility they gave me to attend this University and to obtain the Degree. This accomplishment would not have been possible without them. Thank you.

*Index *

**I**

**NDEX**Abstract ... I Acknowledgements ... II Index ... I Introduction ... 1

Notation and Symbols ... 4

Acronyms List ... 5

1 History of Electromagnetic Absorbers ... 6

1.1Salisbury Screen ... 8

1.2Dallenbach Layer Absorber ... 13

1.3Jaumann Absorber ... 17

2 Radar Absorbers ... 20

2.1Metamaterials ... 21

2.2Lossy Mediums ... 22

2.3Multi-layer Absorbers ... 28

3 Wideband Absorbers using Frequency Selective Surfaces (FSS) ... 31

3.1High-Impedance Surfaces ... 32

3.2Absorbers Comprising Resistively Loaded HIS ... 38

*Index *

4 Non-Conventional Geometry Based Wideband Absorbers ... 47

4.1Absorbers with Embedded FSS ... 47

4.2Absorbers with Perforated Layers and Embedded FSS ... 48

4.3Absorbers with Hilbert and Peano Curve FSS... 50

5 Wideband Absorbers using Commercial Lossy Materials ... 61

5.1Lossy Materials Manufactured by Emerson & Cuming ... 62

5.2Multi-layer Absorbers with Commercial Lossy Materials ... 66

5.32-Layer Optimized Absorber with Commercial Sheets ... 69

5.42-Layer Optimized Absorber with Commercial Materials ... 78

Conclusion ... 83

*Introduction *

**I**

**NTRODUCTION**

Certainly everyone, at least once in life, has thought how it is possible that a military airplane can fly and maybe can attack and destroy a target not being seen on the radar. As it is globally known, the classic purpose of a radar is to find, localize and track a target. But as far as the interest is concentrated in the improvement of the radar performance, in parallel there is the awareness on the techniques to avoid the detection and the tracking of military flying objects. There are few methods that permit to an entity to be not visible on the radar screen, and one of the most studied and discussed regards the electromagnetic absorption theory. In the last years, a considerable part of the research activity in applied electromagnetism has been devoted to electromagnetic absorbing materials. There are many real-world situations where it is necessary to reduce the scattered field by a metallic object, not only in military scenarios. The most intuitive approach to reduce the Radar Cross Section (RCS) of a metallic surface is to cover it with an absorber material which can convert the power into heat. In nature, it is very unusual to find a material with these characteristics and it follows that the studies and the research activities have focused on the invention of new composite materials that can provide this kind of properties. Not all the radars work at the same frequency, in fact there are nine frequency ranges defined in the IEEE 521-2012 that covers from 1 GHz to 110 GHz. Actually, most of the radars use one of the ranges between 2 GHz and 20 GHz and, since the working frequency of the signal which could illuminate the object is not predictable, a wideband absorber is needed. The microwave absorbers for RCS reduction are usually used to coat an object and, for this reason, they need to have suitable characteristics such as light weight, shallow profile, high structural strength and chemical resistance, as well as good absorbing performance. In the design of a radar absorber the thickness of the total structure is very important since the

*Introduction *
absorbing materials need to comply with aerodynamic constraints. For these
reasons a good radar absorbed has to be thin, wideband and lightweight.

The thesis is organized as follow. In the first chapter it is presented an overview on the history of the electromagnetic absorbers, with some details on the concepts and on the theory that allowed Salisbury, Dallenbach and Jaumann to design the first examples of absorbers.

A more detailed definition and description of the materials used in the radar absorbers and the characteristics that define a metamaterial are discussed in chapter two. Some examples and the results of multi-layered structures proposed in literature are shown too.

The third chapter presents the use of Frequency Selective Surfaces in order to realize High-Impedance Surfaces and shows how they can be used in the design of a thin wideband absorbers. Some examples are reported.

In chapter four some non-conventional approaches available in the literature to synthesize wideband absorbers are discussed, and a new design based on the use of a Hamiltonian Curve shape FSS in a double layer structure is proposed.

In chapter five a practical approach to design an absorber based on database of commercial magneto-electric materials with dispersive properties is presented. Frequently, in the literature, materials with ideal properties or hardly reproducible composites are employed in the absorber design. Sometimes no sufficient information on the chemical composition and the manufacturing process of materials is provided and reproducibility of the presented composites is questionable. On the contrary, the use of commercial lossy materials relies on lossy layers are easily available in the market and the electromagnetic characteristics are certified by the manufacturer. Several materials from the Eccosorb® line by Emerson and Cuming are employed in the optimization process and one combination is chosen to design a thin wideband radar absorber.

*Notation and Symbols *

**N**

**OTATION AND**

**S**

**YMBOLS**

The explanations of the notations and symbols used in this dissertation are included as follows:

**E = electric field intensity **
**H = magnetic field intensity **

**η = intrinsic impedance of the medium **
**J = electric current density **

**M = magnetic current density **
**σ = conductivity of the medium **

**λ = wavelength of the electromagnetic wave **

**Γ = reflection coefficient at a certain interface of a system **

**Z = intrinsic impedance of a medium, or seen from an interface **
**Y = intrinsic admittance of a medium, or seen from an interface **
**P = electromagnetic power **

**R = resistance of a component or the entire system **
**k = wave number of the electromagnetic wave **
**ε = permittivity of the medium **

*Acronyms List *

**A**

**CRONYMS**

**L**

**IST**

**AMC: Artificial Magnetic Conductor ****CB: Carbon Black **

**CNF: Carbon Nano Fiber **

**EMA: Electromagnetic Absorption ****FEM: Finite Element Method ****FSS: Frequency Selective Surface ****GA: Genetic Algorithm **

**GNP: Graphene Nano-Platelets ****HIS: High Impedance Surface **

**MWNT: Multi-wall Carbon Nano Tube ****NF: Nano Flakes **

**NP: Nano Particles **

**PEC: Perfect Electric Conductor ****PMC: Perfect Magnetic Conductor ****RA: Radar Absorber **

**RAM: Radiation Absorbing Material ****RCS: Radar Cross-Section **

**Chapter 1- History of Electromagnetic Absorbers **

*C*

*HAPTER *

## 1

**1 **

**H**

**ISTORY OF**

**E**

**LECTROMAGNETIC**

**A**

**BSORBERS**

This chapter shows the most popular absorber designs available in the literature. In order to understand the main characteristics that impact the absorption performance of an electromagnetic absorber, we can evaluate the normalized reflected power level, defined as follows

### 1 (

### )

*absorbed* *reflected* *transmitted*

*P*

###

*P*

###

*P*

_{ }

_{(1.1) }

When the RAM is backed by a metallic surface (PEC plane), there is no transmitted power, and it follows that

### 1

*absorbed* *reflected*

*P*

###

*P*

(1.2)
The objective in designing a good absorber is to minimize the reflected power in a large portion of the spectrum, either in case of normal or oblique incident field angle.

Usually absorption/reflection/transmission coefficients are used instead of power to analyze the performance of the structure.

**Chapter 1- History of Electromagnetic Absorbers **

**Figure 1.1 Geometry of a plane wave passing through two different mediums **

Referring to Figure 1.1, the reflection coefficient can be defined as [1] [2]

0
0 0
0
2 2
0 0
0 0
( )
*jk z*
*jk z* *jk z*
*E*
*jk z*
*E e* *E*
*z* *e* *e*
*E e* *E*
(1.3)
where

*E*

0
and *E*

0
are the amplitudes of the incident and reflected electric fields
*respectively and k is the wave number of the electromagnetic wave in the medium, *
defined as
0,1
0,1
2
*k*
(1.4)

It is evident from (1.3) that the magnitude of the reflection coefficient does not
*depend on z and its phase has a periodicity of λ/2. It is also obvious that *

###

*E*is always

**Chapter 1- History of Electromagnetic Absorbers **

The transmission coefficient can be defined as

0
0
1 1
0 0
( )
*jk z*
*E*
*jk z*
*E e* *E*
*z*
*E e* *E*
_{} _{} _{} (1.5)

As in the case of the reflection coefficient,

###

*E*is always lower than 1 and is

*independent of z. *

In general, the performance of an absorber is measured referring to the reflection coefficient, which can be calculated analytically with the full knowledge of the material profile, or by measuring it in an anechoic chamber.

**1.1 Salisbury Screen **

**1.1 Salisbury Screen**

The Salisbury Screen is one of the oldest and simplest designs for electromagnetic
absorbers. It is realized by placing an infinitesimally thin resistive sheet, with conductivity
*σ, on a low dielectric constant layer backed by a metallic ground plane as shown in *Figure
1.2.

*The thickness of the dielectric layer is d and typically this medium is composed by a plastic *

foam to obtain a relative dielectric constant

###

*r*in the range 1.03 ~ 1.1 .

Referring to the geometry in Figure 1.2 and to the basic electromagnetic theory, the electric

and magnetic fields in the two mediums can be written as:

𝐸0 = 𝐴0+ 𝑒−𝑗𝑘0𝑧+ 𝐴−0 𝑒+𝑗𝑘0𝑧 (1.6)

𝐻_{0} = 1

**Chapter 1- History of Electromagnetic Absorbers **

𝐸1 = 𝐴1+ 𝑒−𝑗𝑘1𝑧+ 𝐴1− 𝑒+𝑗𝑘1𝑧 (1.8)

𝐻_{1} = 1

η_{1} (𝐴1+ 𝑒−𝑗𝑘1𝑧+ 𝐴1− 𝑒+𝑗𝑘1𝑧) (1.9)

**Figure 1.2 Geometry of Salisbury Screen Absorber **

where 𝜂 is the intrinsic impedance of the medium, *A*0,1,

are the amplitudes of the propagating waves.

In order to simplify the analysis, we can consider the plastic foam very similar to the free space, and in this case

*k*

0 ###

*k*

1 and ###

0###

1.The main goal of the structure is to achieve the maximum absorption, and it can be obtained if a destructive interference of the two waves is verified on the interface between the mediums (0) and (1).

**Chapter 1- History of Electromagnetic Absorbers **

0 1

*J*

###

###

*E*

###

*E*

_{ }

_{(1.10) }

0 1

*J*

###

*H*

###

*H*

_{ }

_{(1.11) }

and using the field equations with them, the amplitude of the reflected wave can be written as

###

###

###

###

0 0 0 0 0 2 0 2*jk d*

*jk d*

*jk d*

*e*

*A*

###

*e*

###

*e*

_{ }

_{}

_{ }

_{ }

_{} (1.12)

Looking at (1.12) it is simple to see that at the structure interface the amplitude of the waves must be equal in amplitude and the phase angle must be in opposition. The condition on the amplitude forces σ to be equal to 1/

###

0 , which means that thecharacteristic surface resistance must be 377 Ω/sq.

Under this assumption, the amplitude of the reflected wave on the interface
becomes
0 0
0 0
0
2
cos(k ) cos
*jk d* *jk d* *d*
*A* *e* *d* *e*
_{ } _{} _{ } _{}
(1.13)

Therefore to obtain the maximum absorption, the (1.13) must be equal to zero, which implies

0 0 _{0,1, 2,...}

4 2

*d* *n* *n* (1.14)

Considering a more general case, where the spacer is a generic dielectric layer (

*k*

0###

*k*

1 and ###

0###

1), the amplitude of the reflected wave reads:* Chapter 1- History of Electromagnetic Absorbers *
0
1 1
0 0
0 0 0
1 1
1 1
2

*jk d*

*jk d*

*jk d*

*e*

*A*

###

###

*e*

###

###

*e*

###

###

_{ }

_{ }

_{}

_{}

_{ }

_{} (1.15)

Similarly to the previous case, to have maximum absorption, the two exponentials must have the same amplitude and opposite phase angle:

0 0
0 0
1 1
1 1
_{ } _{ }
(1.16)

Consequently relation (1.15) becomes

0 0 0 0
0 1
1 1 1
2
cos(k ) cos
*jk d* *jk d* *d*
*A* *e* *d* *e*
_{ } _{} _{} _{ } _{} _{}
(1.17)

As in the previous case, this amplitude should be equal to zero, which implies:

1 1 _{0,1, 2,...}

4 2

*d* *n* *n* (1.18)

Therefore, in the design of a Salisbury Screen absorber, it is possible to use different
materials as dielectric substrate. Usually, high values of permittivity are employed
to have strong and sturdy structures. The final results show that the thickness of the
Salisbury Screen can be modified by using different dielectrics, because the
*minimum value of d correspond to a quarter of the specific wavelength of the *
material. Figure 1.3 shows the performance of a Salisbury Screen with a 7.5 mm air
layer between the resistive sheet and the PEC backing using different values of
resistive sheets. According to (1.18) the maximum absorption deep is exactly at 10
*GHz (λ = 30 mm) and the best performance is achieved with a resistivity of 377 Ω/sq *
reaching a magnitude of the reflection coefficient lower than – 70 dB.

**Chapter 1- History of Electromagnetic Absorbers ****-80**
**-70**
**-60**
**-50**
**-40**
**-30**
**-20**
**-10**
**0**
**2** **4** **6** **8** **10** **12** **14** **16** **18** **20**

**Salisbury Screen with Different Sheet Resistances**

**Rs = 377**
**Rs = 100**
**Rs = 300**
**Rs = 500**
**Rs = 600**
**R**
**e**
**fl**
**e**
**cti**
**o**
**n**
** C**
**o**
**eff**
**ici**
**en**
**t **
**[d**
**B**
**]**
**Frequency [GHz]**

**Figure 1.3 Reflection Coefficients for a Salisbury Screen with d = 7.5 mm with different **

*sheet resistances *

Acceptable performance is also visible with a sheet resistance of 300 Ω/sq where the minimum of the reflection coefficient reaches – 18.9 dB. It is important to notice that, according to (1.17), the frequency position of the absorption deep is fixed when sheet resistance is changing, because it is related only to the thickness of the spacer and on the characteristics of the material.

The use of different dielectric spacers, as can be seen in Figure 1.4, does not modify the frequency position of the deep which is still at 10 GHz, but it induces a reduction in the absorption bandwidth.

**Chapter 1- History of Electromagnetic Absorbers ****-80**
**-70**
**-60**
**-50**
**-40**
**-30**
**-20**
**-10**
**0**
**8** **10** **12**

**Salisbury Screen with Different Dielectric Spacers**

**Eps = 1**
**Eps = 9**
**Eps = 25**
**R**
**e**
**fl**
**e**
**c**
**tio**
**n**
** Co**
**e**
**ff**
**ic**
**ie**
**nt**
** [**
**d**
**B**
**]**
**Frequency [GHz]**

**Figure 1.4 Reflection Coefficients for a Salisbury Screen with d = 7.5 mm with different **

*materials used for the spacer *

**1.2 Dallenbach Layer Absorber **

**1.2 Dallenbach Layer Absorber**

A homogeneous lossy layer with dielectric and magnetic properties backed by a metallic plate can be also used as an absorber. This configuration is called Dallenbach Layer Absorber and shown in Figure 1.5 .

As a general concept, in the case of a wave passing through different mediums, the change of the impedance seen by the wave at the surface causes the reflection. The basic idea for this absorber is to find a material whose impedance relative to free space is equal to 1, which yields no reflection at the interface. However, it is difficult to find a material with appropriate dielectric and magnetic properties, which can

**Chapter 1- History of Electromagnetic Absorbers **

act as a perfectly matched RAM. Generally, the total absorption is related to the loss properties of the material and the electrical thickness. Thus the main goal becomes to optimize the total loss at a given frequency using available materials.

**Figure 1.5 Geometry of Dallenbach Layer Absorber **

Analyzing the geometry in Figure 1.5, the reflection coefficient

###

is given by [1], [2] 0 0*in*

*in*

*Z*

*Z*

*Z*

*Z* (1.19)

where

*Z*

0 is the intrinsic impedance of free space and *Z*

*in*, given by

###

###

###

###

tan tan*L*

*m*

*d*

*in*

*m*

*m*

*L*

*d*

*Z*

*jZ*

*k d*

*Z*

*Z*

*Z*

*jZ*

*k d* (1.20)

**Chapter 1- History of Electromagnetic Absorbers **

represents the impedance seen by the wave at the interface of the absorber,

*Z*

*L*is the

intrinsic impedance of the load, and

*Z*

*m*is the impedance of the material used for

the layer
*d*
*m*
*d*
*Z*
(1.21)

In this case the load is a metallic plane and the impedance is essentially 0, which yields to

###

###

_{}

_{}

tan
tan
*m*

*d*

*PEC*

*in*

*d*

*m*

*m*

*d*

*m*

*jZ*

*k d*

*Z*

*Z*

*Z*

*jZ*

*k d*

*Z* (1.22) and consequently

###

###

###

###

00 0 0 2 tan 1 tan tan 2 tan 1*d*

*d*

*d*

*d*

*m*

*d*

*m*

*d*

*d*

*d*

*d*

*d*

*d*

*j*

*jZ*

*k d*

*Z*

*jZ*

*k d*

*Z*

*d*

*j*

_{ }

_{ }

_{}

_{}

_{}

_{}

_{}

_{} (1.23)

From the (1.23) it is evident that with the knowledge of the permittivity and permeability of the lossy material used for the Dallenbach Layer Absorber, the absorption performance of the structure depends only on the thickness of the layer. In this structure, due to the potentially dispersive nature of the permittivity and permeability profile of the lossy layer, the optimal choice of the layer thickness does not follow the quarter-wavelength rule, and furthermore an increase in the thickness of the lossy material does not guarantee a shift of the absorption peak. Figure 1.6 shows the reflection coefficient for a Dallenbach Layer absorber with different thicknesses using as a lossy material the Eccosorb SF2 produced by Emerson & Cuming.

**Chapter 1- History of Electromagnetic Absorbers ****-35**
**-30**
**-25**
**-20**
**-15**
**-10**
**-5**
**0**
**2** **4** **6** **8** **10** **12** **14** **16** **18** **20**

**Dallenbach Layer Absorber with Eccosorb SF2**

**d = 1 mm**
**d = 2 mm**
**d = 3 mm**
**d = 4 mm**
**d = 5 mm**
**R**
**e**
**fl**
**e**
**c**
**ti**
**o**
**n**
** Co**
**e**
**ff**
**ic**
**ie**
**nt**
** [**
**d**
**B**
**]**
**Frequency [GHz]**

**Figure 1.6 Reflection Coefficient for a Dallenbach Layer Absorber with different **

*thicknesses *

The electromagnetic properties of this material are shown in Figure 1.7 and it can
be found on the commercial market in the form of thin layers with fixed thicknesses.
*In this case the change of d causes the shift of the main absorption deep towards *
lower frequencies despite the magnitude value of the reflection coefficient becomes
lower in absolute terms.

**Chapter 1- History of Electromagnetic Absorbers ***(a) *
**25.99**
**26**
**26**
**26.01**
**26.01**
**26.02**
**2** **4** **6** **8** **10** **12** **14** **16** **18** **20**
**Eccosorb SF2**
**Re**
**al **
**Par**
**t of**
** P**
**er**
**m**
**itt**
**ivi**
**ty**
**Frequency [GHz]**
*(b) *
**0**
**1**
**2**
**3**
**4**
**5**
**6**
**7**
**2** **4** **6** **8** **10** **12** **14** **16** **18** **20**
**Eccosorb SF2**
**Re**
**al **
**Pa**
**rt of **
**Perm**
**ea**
**b**
**ili**
**ty**
**Frequency [GHz]**
*(c) *
**0.25**
**0.3**
**0.35**
**0.4**
**0.45**
**0.5**
**0.55**
**0.6**
**2** **4** **6** **8** **10** **12** **14** **16** **18** **20**
**Eccosorb SF2**
**Ima**
**g**
**inar**
**y Pa**
**rt **
**o**
**f Pe**
**rmitt**
**iv**
**ity**
**Frequency [GHz]**
*(d) *
**1**
**1.2**
**1.4**
**1.6**
**1.8**
**2**
**2.2**
**2.4**
**2.6**
**2** **4** **6** **8** **10** **12** **14** **16** **18** **20**
**Eccosorb SF2**
**Ima**
**g**
**in**
**ar**
**y Pa**
**rt **
**o**
**f **
**Per**
**mea**
**b**
**il**
**it**
**y**
**Frequency [GHz]**

**Figure 1.7 Electromagnetic properties of commercial Eccosorb SF2: (a) real part of **

*Permittivity, (b) real part of Permeability, (c) imaginary part of Permittivity, *
*(d) imaginary part of Permeability *

**1.3 Jaumann Absorber **

**1.3 Jaumann Absorber**

When dealing with electromagnetic absorbing materials, other than the levels of absorption, another characteristic that is very important and must be evaluated is the absorption bandwidth. Usually the requirements of the project indicate a frequency band where the value in decibel of the reflection coefficient should be lower than a certain threshold (-10 dB is a common value). Often absorbers are used in military scenarios, which means that they have to cover the radar bandwidth (2 GHz - 18 GHz) and their performance are supposed to deteriorate slowly out of this frequency range. Figure 1.4 shows that the Salisbury Screen cannot cover the full

**Chapter 1- History of Electromagnetic Absorbers **

radar bandwidth, but the coverage can be improved by adding other dielectric layers and resistive sheets [4]. This structure is known as Jaumann Absorber (Figure 1.8).

**Figure 1.8 Geometry of Jaumann Absorber **

An example of the reflection coefficient of a Jaumann Absorber with eight layers made of the same material, is shown in Figure 1.9. The thicknesses and the sheet resistances are shown in Table 1 and Table 2 respectively.

**Table 1 Thicknesses for the layers of the Jaumann Absorber [mm] **

*d1 * *d2* *d3* *d4 * *d5* *d6* *d7* *d8*

**Chapter 1- History of Electromagnetic Absorbers **

* Table 2 Sheet Resistances for the layers of the Jaumann Absorber [ *

_{sq}]The simulated reflection coefficient for this absorber has a -10 dB absorption
bandwidth of 2 – 36.2 GHz and a -20 dB absorption bandwidth of 3 - 35.2 GHz in
the case of air or similar material as filler of the layers. The total thickness of this
absorber is 31.4 mm, slightly larger than a quarter of wavelength at the lower
frequency (3 GHz). The performance for this absorber can be considered as
ultra-wideband, but the total thickness is too large to consider it as thin layer. Alternative
approaches need to be considered to reduce the thickness while maintaining the
same performance.
**-40**
**-35**
**-30**
**-25**
**-20**
**-15**
**-10**
**-5**
**0**
**0** **5** **10** **15** **20** **25** **30** **35** **40**

**Jaumann Absorber with 8 layers**

Er = 1
Er = 9
Er = 25
**R**
**e**
**fl**
**e**
**c**
**ti**
**o**
**n**
** C**
**o**
**e**
**ff**
**icien**
**t **
**[d**
**B**
**]**
**Frequency [GHz]**

* Figure 1.9 Reflection Coefficient of Jaumann Absorber with different permittivity *
1

*S*

*R*

*2*

*S*

*R*

3
*S*

*R*

4
*S*

*R*

5
*S*

*R*

6
*S*

*R*

7
*S*

*R*

8
*S*

*R*

305 579 873 1266.5 1796 2480 3724 2067
**Chapter 2- Radar Absorbers **

*C*

*HAPTER *

## 2

**2 **

**R**

**ADAR**

**A**

**BSORBERS**

In this chapter the basic concepts and the characteristics of the materials used to design an electromagnetic absorber are discussed, focusing on some ad-hoc proposed materials.

As is well known, the radar theory is based on the Maxwell equations and on the EM waves propagation. The basic concept used by the classic radar is the following: when the power radiated from an antenna impinges an object, some reflection occurs and some reflected power comes back to the radar antenna. By analyzing the parameters associated to this incoming wave, it is possible to generate an image of the object and in case of moving items it can also be predicted its speed and its trajectory.

In parallel with the development of the radar theory, the research activity finalized to make an object invisible to the radars was developed mainly in the military field. Since the World War II, one of the most studied methods to have no power going back to the radar antenna, which is also the basis of this work, is to coat an object with a sort of material able to absorb all the electromagnetic waves incident on its surface. One of the official first examples of this “invisible objects” was the stealth aircraft, developed by different companies in different versions. Actually no aircraft is totally invisible to radars, but stealth aircrafts are difficult to detect or track for

**Chapter 2- Radar Absorbers **

they use some active measures and emitters employed to reduce the EM emissions and interfering with the coded signal used by the radar.

In this work we will discuss about the possibility of designing a radar absorber, on a band ranging from 2 to 18 GHz, using commercial lossy materials in a layered structure similar to the Jaumann configuration. The choice of commercial materials is not common in literature, since the use of ad-hoc materials synthetized in a chemical laboratory are frequently proposed in order to obtain a specific electromagnetic behavior. One of the problems of these materials is that, even if the whole procedure to create them is described, it is almost impossible to obtain the same electromagnetic characteristics when trying to make them in another laboratory.

For these reasons, the focus of this work is to try to design an absorber employing commercial materials, simply available and with properties certified by the manufacturer.

The main goal of a radar absorber is to suppress the reflected energy generated by the incident wave on the surface of the structure, by dissipating the magnetic and/or electrical fields into heat. The absorbers can be divided into magnetic and dielectric absorbers, according to their lossy fillers. The magnetic ones are usually used as coating materials and the fillers are made by mixing rubbers or polymeric resins with compounds of relatively heavy metals or ceramic, mostly used at high mixing ratios. The conductive fillers are used to control the complex permittivity only.

**2.1 Metamaterials **

**2.1 Metamaterials**

The studies and the experiments on artificial materials for manipulating waves
began at the end of 19th_{ century, defining the first examples of metamaterials [5], but }
a more specific definition of metamaterials emerged about 50 years later [6] , [7].

**Chapter 2- Radar Absorbers **

A metamaterial is an artificial material designed to have properties that any other material has in nature [8], [9], [10]. The use of a metamaterial allows to block, to enhance, to bend or to enhance waves achieving advantages that are not attainable with common materials. Metamaterials can be realized by assembling multiple materials (metals or plastic) or combining different layers of materials or working on single elements chemically. The structure of metamaterials is usually arranged in repeating patterns and their properties do not come from the characteristic of the base material, but it is the specific shape, the orientation, the size and the geometry that give them the capacity of manipulating electromagnetic waves.

Metamaterials have several and various potential interdisciplinary applications, including optical filters, remote aerospace applications, sensor detection, radomes, high-frequency battlefield communication and lenses for high-gain antennas [11], and even shielding structures [12] , [13]. In the modern electromagnetic theory metamaterials are also used to design microwave absorbers [14], [15], [16].

**2.2 Lossy Mediums **

**2.2 Lossy Mediums**

Each material has electromagnetic properties that play a key role in determining the
performance in term of reflection and attenuation for an absorbing structure. The
permittivity *r* is the measure of resistance that is encountered when forming an

electric field in a medium and the permeability *r* is the measure of the ability of a

material to support the formation of a magnetic field within itself. Each of these parameters is a complex quantity, which yields

' ''
*r*

*j*

###

###

###

(2.1) ' ''*j*

###

###

###

(2.2)**Chapter 2- Radar Absorbers **

where all the values are normalized by the values of the free space 0 and 0. The

imaginary part of permeability and permittivity is strictly connected to the loss in
the medium. Referring to these properties, we can define lossy materials the ones
with *r* 1 and

''

0 .

The loss in a material is also generated by the electric conductivity of the material that contributes to imaginary part of permittivity ''

:

'' 0

###

###

(2.3)Experimental results show that the loss effect connected to the permittivity is much lower than the one generated by the permeability, and the absorber thickness is more affected by the real part of the complex permittivity than the imaginary part. It is found that the reflection and attenuation performance of an absorber depends on six characteristic parameters, as can be seen in (1.23): the wavelength

###

, the*thickness d and the real and imaginary part of*

*r*and

*r*. Therefore fixing the

frequency and the thickness, the only way to obtain it is to work on the combination
of *r* and *r*[17].

One of the most used compound classified as lossy medium is the ferrite; it is usually composed of iron oxide combined chemically with one or more metallic elements. The proportion between the basic elements of the compound determinates the different electromagnetic characteristics of the medium and it follows a change of the absorption characteristics of the absorber.

In order to generate a good loss level, the ferrite can be mixed with different materials as for instance, rubber [18]. This particular composite, as many others, has a narrowband response if used as layer in a classic Dallenbach configuration. It is shown that increasing the mixing ratio of ferrite to rubber, the absorption deep moves to higher frequencies even if the minimum value of magnitude does not

**Chapter 2- Radar Absorbers **

follow a specific scheme as well. It is also demonstrable that the higher value of

###

*r*'

,

###

*r*' and tan

###

induces the thinner absorber. There are multiple solutions to create composite laminates that can be used in the design of electromagnetic absorbers. In [19] an E-glass/epoxy composite laminate containing three types of carbon nano materials has been studied, expecting to have a different effect on the value of the real and the imaginary part of the complex permittivity.

*Kim et al. [19] used carbon black (CB), carbon nano fiber (CNF) and multi-wall *
carbon nano tube (MWNT), trying different concentrations of the filler to study the
behaviour of the composite. Referring to Figure 2.1, it is evident that the three types
of carbon nano materials have a different atomic structure that generates the proper
electromagnetic characteristics of each of them.

**Figure 2.1 Scanning electron photos of the carbon black (CB), carbon nano fiber (CNF) **

*and multi-wall carbon nano tube (MWNT) [19] *

In [20] flake-like particles are employed. Having a higher shape anisotropy compared to sphere-like particles, more convenient values of complex permittivity and permeability can be obtained. Physically speaking, due to the high surface-to-volume ratio, the flake-like particles interface area is greatly larger compared to the sphere-like particles and it follows that theoretically the loss can be higher. CoFe alloy Nano-Flakes (NFs) and Nano-Particles (NPs) were prepared with hydrogen-thermal reduction method and the electromagnetic parameters were measured on

**Chapter 2- Radar Absorbers **

a Vector Network Analyser (VNA) on transmission/reflection mode. The measured permittivity and permeability of the composite specimens are shown in Figure 2.2, and it is visible that the EM characteristics of CoFe alloy NFs look more lossy than the NPs ones, in fact the imaginary part of NFs permittivity is high and infers an intense dielectric loss compared to NPs.

A physical reason for higher

###

*r*' of CoFe alloy NFs is that in the gigahertz frequency

band, the dynamic magnetic properties for high conductivity particles are strictly connected to the eddy current and the loss on the permeability in NFs is more effectively suppressed than that in the case of CoFe alloy NPs.

**Figure 2.2 Complex Permittivity (a) and Complex Permeability (b) of composites specimen **

*measured on a bandwidth of 2-18 GHz [20] *

Lots of research works are now focused on the chemical study of lossy materials. Starting from the proposed alloys, they combine or add some elements, or they modify the producing process in order to obtain different electromagnetic characteristics for the final material. Ultimately, the main goal seems to be to produce materials in which the particles have a high surface-to-volume ratio and a low conductivity, and thus suppress the eddy current effect improving the permeability of the composite.

**Chapter 2- Radar Absorbers **

Most of the conclusions of previous works on metamaterials show that it is very difficult to achieve a good absorption performance on a wide frequency band only using one layer of lossy material backed by a metal plane. As well known, to obtain a good absorption level, at the incident interface of the structure it is necessary to have the impedance matching, to reduce the reflected power and to maximize the power that propagates into the layers. Afterwards, we need high dielectric or magnetic dissipation in the filler material to have less power as possible coming back out of the structure after the reflection on the metal plane. The main problem seems to be the difficulty to find a good equilibrium between dissipation and impedance matching using only one material, if a working bandwidth wide as the radar one is desired. Usually, natural materials have a permeability lower than permittivity, so magnetic material such as ferromagnetic alloys could be used in the design of an absorber structure mainly for the matching purpose.

In [21] the use of a dual layer absorber is proposed to be a reasonable solution to obtain the impedance matching on the outer layer and the power dissipation in the inner layer on a wide frequency band. In the top substrate CoFe3/Al2O3 is utilized as filler, because it is shown that it prevents the agglomeration during the reduction process and it allows the particle size to be enlarged, and CoFe NFs are adopted as fillers in the absorbing layer. The thicknesses of the layers, following a classic approach in these cases, are optimized by using a GA method to obtain the widest reachable absorption performance.

The experimental results show that the effective bandwidth obtained with the dual-layer structure is greatly wider than the one using only one CoFe alloy NFs dual-layer (Figure 2.3), which means that a good impedance matching characteristic is achieved by CoFe3/Al2O3 composite nanoparticles. In this structure, the reflection coefficient remains less than -10 dB on the frequency range from 2.5-18 GHz, and less than -15 dB on the band of 5-15 GHz, actually a not predictable behaviour analysing and combining the ones of the single layer case.

**Chapter 2- Radar Absorbers **

**Figure 2.3 EMA performance of dual-layer absorber backed with PEC plate [21] **

Going forward through the idea of improving the surface-to-volume ratio, we can mention the use of carbon nano-tubes in the composites for EM applications. Then the evolution can be seen in graphite nano-platelets (GNPs), which are presented in [22]. One of the most interesting aspects of these particles is that they can be dispersed in a polymeric matrix, increasing in this way the loss of a material block or even locally only in a specific area of a layer. The electromagnetic properties of this drugged material can be calculated analytically and therefore controlled through the manufacturing process. Nano-platelets can also be deposited on the surface of a material and seen as a bi-dimensional sheet that can be stacked up above other layers to obtain a more complex structure.

*Gaetano et al. [22] propose the use of GNPs composites in a shielding multilayer *
structure without metallic planes, that offers a -10 dB reflectivity on a band from 2
to 18 GHz with a wave incident on the top side, or a frequency range from 3.6 to
18 GHz with a wave incident from the down side.

**Chapter 2- Radar Absorbers **

**2.3 Multi-layer Absorbers **

**2.3 Multi-layer Absorbers**

The simplest electromagnetic absorber is a single layer of dielectric or lossy material backed by a metallic plane. In real situations, this structure is used to coat a metallic object (that represents the PEC plane). An efficient way to improve the performance of the absorber is to add more layers and elements to the structure.

In [23] it is demonstrated the least thickness to bandwidth ratio achievable for a physically realizable radar absorber, which is one of the foundation of the actual theory on the absorbers.

When designing a microwave absorber, we have to think that the actual scenario is mostly military, which means that we have to satisfy some requirements. We should have the minimum possible thickness, because adding some material to coat an aircraft means an increase of weight and thus more use of fuel and worse flying performance. We also should have the best possible performance, namely the lowest possible reflectance, and the widest operating bandwidth, but all these requirements are conflicting to each other.

Ideally if we could use a material with a frequency dependence of the permeability and permittivity that can be selected arbitrarily, we could achieve the maximum absorption on the desired bandwidth without considering the thickness of the layer. This would be the basic idea for a perfect radar absorber. In real materials, real and imaginary part of permeability and permittivity are correlated to each other by means of the Kramers-Kronig relations, and it means that the operating bandwidth of a single lossy layer is limited. In some cases, such as a single layer absorbing structure (Dallenbach screen), it is also possible to calculate the analytical equation that define a relation between thickness of the layer, the electromagnetic characteristics of the material and the operating bandwidth. As is well known, the performance of this type of absorber can be improved by increasing the permeability of the medium. However, the permeability of known lossy materials

**Chapter 2- Radar Absorbers **

is usually too low to obtain good absorption performance, and it follows the interest into multilayer structures and metamaterials. Unfortunately, no analytical expressions on the working bandwidth are available for these cases and the usual approach consist of the optimization of the performance by using parametrized simulations. These numerical methods can provide the upper bound for the thickness to bandwidth ratio of the absorbers.

Rozanov [23] defines, for the case of any metal-blocked magnetodielectric layer, the analytical relation between the reflection coefficient ( ) , the thickness of the slab

and its static permeability, defined as

'

*S* _{}

(2.4)

Under the condition of the wavelengths tending to infinity, any thickness of the material is small compared to

###

, which yields to2

0 ln ( ) d 2 *Sd*

###

(2.5)And for the case of a multilayer structure we have

2
0 ln ( ) d 2 *Si* *i*
*i*
*d*

###

###

###

###

###

(2.6)where

###

*S*and

_{i}*di are the static permeability and the thickness of the ith layer*

respectively.

When applying the (2.6) to a generic radar scenario, we can analyze the case when the reflection coefficient of a radar absorber is less than 0 within the operating

**Chapter 2- Radar Absorbers **

###

###

2 0 max min ln 2*i*

*S*

*i*

*i*

*d*

###

(2.7)Inequality (2.7) can be used to estimate the largest possible bandwidth we can achieve with a prescribed thickness and reflection coefficient of the absorber. At the moment inequalities (2.5), (2.6) and consequently (2.7) are considered the actual limit for the thickness to bandwidth ratio achievable for a physically realizable radar absorber. Even if in [23] it is indicated the possibility to have a thickness in real absorber less than the one calculated with (2.6), in literature no one has been able to design or to realize an absorber with a thickness smaller than the predicted one. Thus this limit is also used to compare proposed results, considering it the optimum value that can be obtained.

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

*C*

*HAPTER *

## 3

**3 **

**W**

**IDEBAND**

**A**

**BSORBERS**

**USING**

**F**

**REQUENCY**

**S**

**ELECTIVE**

**S**

**URFACES**

**(FSS) **

This chapter presents one of the modern design approaches for electromagnetic absorbers. It is based on FSS (Frequency Selective Surfaces). The FSS layer, analogously to Salisbury or Jaumann absorbers, is printed above a dielectric substrate with a PEC backing and it is used as a resonant structure to match a specific frequency. The FSS is employed in place of a uniform resistive sheet as it can provide complex surface impedance instead of only resistive impedance. This characteristic allows achieving an improved versatility in designing electromagnetic absorbers. Working with resonant structures, the absorption performance of thin absorbers employing FSS is narrowband. Usually an absorber is used to cover big surfaces or objects, but in the radar bandwidth (Gigahertz frequencies), the wavelength

###

goes from 1 cm to 30 cm and it means that only one resonant structure, normally with dimensions of / 4 , is not enough to fill the whole surface of interest. Accordingly, a periodic array or a matrix of FSS is used and the resonant frequency of the screen is determined by the size, the shape and the resistivity of the metal used to print the single unit cell. One way to increase the working bandwidth of the absorber is to produce multiple resonances among the**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

grounded dielectric slab and the FSS or to design the unit cell of the FSS with multiple resonances.

Some examples of FSS-based absorber are presented in this chapter, to show how from different primary concerns follow different approaches and designs for absorbers.

**3.1 High-Impedance Surfaces **

**3.1 High-Impedance Surfaces**

The design of electromagnetic absorbers is mostly based on the choice of the materials for the layers and on their optimal thickness. It is demonstrated that by adding elements to the basic layered structure, it is possible to enlarge the total bandwidth of the absorber, combining in this way different adjacent resonant frequencies.

The use of High-Impedance Surfaces (HIS) in electromagnetic devices is common, especially because they can mimic the behavior of an ideal Artificial Magnetic Conductor (AMC) on a small frequency range. An AMC is a surface characterized by a reflectivity of +1, and it can also be seen as a Perfect Magnetic Conductor (PMC). This condition means that the phase of the reflection coefficient is zero degrees, or similarly that the reflected wave is in phase with the incident one. Unfortunately, this kind of material does not exist in nature, so the only way to realize it is to use metamaterials. The use of FSS, mainly on the top of a layered structure, is very common to synthetize a HIS (Figure 3.1).

Multiple different shapes of the FSS have been proposed in the literature, basing the
choice of the geometry on an equivalent circuit theory [24] [25] in case of normal
incidence, that allows to size the dimensions in order to have a specific resonance
and a working bandwidth. According to (1.22), the dielectric layer backed by the
*metal plane behaves as an inductor when its thickness d is << *

###

*, with an impedance*

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

*d* *s*

*Z* *j**d* *j**L* (3.1)

where

###

is the permeability of the material used for the layer.**Figure 3.1 3-D example of HIS layered structure **

The FSS can be considered as a pure capacitive element *CFSS* on small frequency

*ranges or as a RLC series circuit for a larger bandwidth. The absorbing structure can *
*be seen as behaving like a parallel LC circuit (Figure 3.2b). As well known, the *
resonant frequency of the circuit *f*0* and the bandwidth BW of the HIS structure are *

0
1
2 _{S}_{FSS}*f*
*L C*
(3.2)
0 0
1 _{S}*FSS*
*L*
*BW*
*Z* *C*
(3.3)

where *LS* is the inductance of the substrate, *Z*0 is the free-space impedance, and 0

* Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) *
0
1

*S*

*FSS*

*L C* (3.4)

Hence, the surface impedance may be represented as

2
0
1
*S*
*R*
*j L*
*Z*
(3.5)

There are different methods to modify the resonant frequency of the structure. The
most obvious one affects simple modifications of the unit cell geometry, by
increasing the printed surface area between adjacent cells, for instance, the
capacitance grow up and from (3.2) it is evident that *f*0 is reduced, maintaining the

same unit cell size and substrate parameters. Furthermore, an increase of the substrate thickness, according to (3.1) and (3.2), produces a lower resonant frequency.

*a) * *b) *

**Figure 3.2 Equivalent Transmission Line circuit of a) high-impedance surface and b) its **

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

In [25] it is demonstrated that modeling the FSS by using only the capacitor is a good tool for studying some particular cases, but it does not allow to evaluate the working bandwidth of the structure. In fact, even if using FSS with different shapes, but with the same value of averaged capacitance, the calculated bandwidth would be always the same.

To evaluate the behavior of the HIS structure in a more general way, it is necessary
to consider a circuit where the FSS is modeled as the series of a capacitance *CFSS* and

an inductance *LFSS*(Figure 3.3).

Basing on this new idea, the impedance of the circuit is

2
2
(1 )
1 ( )
*S* *FSS* *FSS*
*R*
*FSS* *FSS* *S*
*L* *L* *C*
*Z* *j*
*C* *L* *L*
(3.6)
*a) * *b) *

**Figure 3.3 Equivalent Transmission Line circuit of a) high-impedance surface and b) its **

*corresponding lumped circuit model in case of FSS modeled as a series of a capacitor and an *
*inductor *

The high-impedance condition is verified when the denominator of (3.6) is zero, namely when the angular frequency is equal to

* Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) *
0
1
(L )

*FSS*

*FSS*

*S*

*C*

*L* (3.7)

The bandwidth of the new circuit must be referred to the case of a high-impedance
surface, where it is defined as the frequency range where the absolute value of the
impedance is larger than the free-space impedance. Thus, it is necessary to find the
frequencies for which the impedance in (3.6) is equal to *Z*0 and *Z*0.

After some algebra, the final expression of the fractional bandwidth of the new circuit can be expressed as

###

###

###

###

0 0 2 0 2 cos( ) 3 sin( ) 3*Z*

*Z*

*FSS*

*FSS*

*S*

*FBW*

*C*

*L*

*L*

*Q*

*A*

_{}

_{} (3.8) where 0 0

*S*

*FSS*

*FSS*

*Z*

*A*

*L L C* (3.9) 1 1

*FSS*

*FSS*

*A*

*L*

*C* (3.10) 0 2 (

_{S}*)*

_{FSS}*S*

*FSS*

*Z L*

*L*

*A*

*L L* (3.11) 2 1 2 3 9

*A*

*A*

*Q* (3.12) 3 1 2 0 2 9 27 2 54

*A A*

*A*

*A*

*R* (3.13)

* Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) *
1
3
cos

*R*

*Q*

_{}

_{}

_{}

_{} (3.14)

are coefficients calculated or defined during the calculation.

From (3.7) it is evident that the modification of the FSS shape, with the thickness of the dielectric fixed, makes the resonant frequency change. But it is also demonstrated experimentally that the inductance and the capacitance related to the frequency selective surface, are strictly connected and it is not possible to vary one of them without change the other one. In fact, the use of large elements with respect to the unit cell, namely the increase of printed surface between adjacent cells, produces the decrease of the value of the FSS inductance. Eventually it is demonstrated that the fractional bandwidth of the structure can be maximized by decreasing the inductance and consequently increasing the value of the capacitance. According to these results, we expect that a cross element will be the most narrowband, whereas a patch-type element will be the most wideband even if its capacitance is higher.

In [24] it is shown an example on how the use of two different sized squared patch in a specific geometry (Figure 3.4a) generates three different resonant frequencies of the structure. Afterwards, to add more resonances, they modify the smallest square patches, including three additional smaller patches (Figure 3.4b) to form a repetitive, reduced scaled version of the original maintaining the overall unit cell size the same. Keep on repeating this addition, they can obtain FSS shapes like the ones in Figure 3.4c and Figure 3.4d, adding in this way more resonant frequencies to the absorbing structure.

It is also demonstrated in [26] that it is possible to reduce the mutual coupling between the antenna elements, namely suppressing the surface waves, by placing thin strips of AMC between the cells.

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

*a) * *b) * *c) * *d) *

**Figure 3.4 Examples of Geometries used for the Unit Cell of the Periodic Metallic Screen **

*in [24] *

An alternative approach to tune the resonance of the structure is to work on the characteristics of the dielectric substrate and leave unchanged the geometry of the FSS screen. In this case it can be used a tunable dielectric material, that changes its permittivity depending on the applied electric field, hence the resonant frequency can be controlled accordingly.

In literature some simple designs have been presented, also proposing for instance a multilayer structure composed only by FSS with vacuum spacers, analyzing different unit cell shapes [27].

**3.2 Absorbers Comprising Resistively Loaded HIS **

**3.2 Absorbers Comprising Resistively Loaded HIS**

In recent years, the use of frequency selective surfaces and the amount of their possible shapes has been investigated in order to enhance the performance of absorbers. Usually structures with perfectly conductive FSS layers loaded with lumped resistors are employed to synthetize thin and wideband absorbers without following the rule of the quarter-wavelength on the thickness. Alternatively, another approach is to use a resistive or low-conductivity FSS instead of the combination of a conductive layer and lumped resistor. Some rules for the design of resistive loaded High-Impedance Surfaces are presented in [28], but they are mostly referred to wideband cases and a specific theory of narrowband structures is not available. It is also very difficult to find a useful method to choose the most

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

*Costa et al. in [29] present a thin electromagnetic absorber using HIS comprising *
lossy FSS, which can be used as a narrowband or as a wideband absorber, obtaining
in this last configuration -15 dB of the reflection index over a band from 7 to 20 GHz
with a total thickness of the structure of 5 mm (Figure 3.5). The proposed structure
is very simple: a dielectric thin slab backed with a metal plane and on the top there
is a FSS array, made of capacitive cells, with squared elements. Three different cell
shapes have been simulated, a cross, a squared ring and a squared patch to show
how the reflection coefficient changes depending on this choice. The best results, for
the wideband configuration, have been obtained with the third cell shape, namely
with the squared ring (Figure 3.6). This approach is based on the fact that the use of
lumped resistors, finalized to introduce ohmic losses, makes the project to be very
complex and expensive.

**Figure 3.5 Reflection Coefficient of the Absorber proposed in [29] calculated with three **

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

**Figure 3.6 3D geometry of the Absorber proposed in [29] **

The analysis of the behavior of the structure is done using a simple equivalent
circuit, and this idea allows to demonstrate that the optimum surface resistance of
the ink depends on multiple parameters, as the permittivity of the substrate, the
distance of the FSS from the PEC plane, and obviously on the unit cell shape.
Following the concept of the equivalent circuit, the impedance of a lossy FSS can be
represented as
2
1 _{FSS}_{FSS}*FSS*
*FSS*
*L* *C*
*Z* *R* *j*
*C*
(3.15)

where *R*, *LFSS* and *CFSS* represent the elements of the RLC circuit, which depend on

the shape of the FSS. The surface impedance of the absorbing structure *Z _{R}* can be

defined as
/ /
( )
*d* *FSS*
*R* *FSS* *d*
*d* *FSS*
*Z Z*
*Z* *Z* *Z*
*Z* *Z*
(3.16)

where *Zd*is the impedance of the grounded dielectric stub as defined also in (1.22)

tan(k ) *d* tan( )

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

*and where the approximation is valid when d* , which is also identical to (3.1).
In order to obtain the maximum absorption of the incoming wave, we need the
parallel circuit to resonates, and the impedance *ZR* to become purely real.

After some manipulations, the real and the imaginary part of *ZR* can be derived:

###

2 2 2 2 Re 1*d*

*R*

*FSS*

*FSS*

*d*

*FSS*

*RZ*

*Z*

*L*

*C*

*Z*

*R*

*C*

_{}

_{} (3.18)

###

###

###

2 2 2 2 2 2 1 1 Im 1*FSS*

*FSS*

*d*

*FSS*

*FSS*

*FSS*

*d*

*d*

*d*

*d*

*FSS*

*FSS*

*FSS*

*R*

*FSS*

*FSS*

*d*

*FSS*

*L C*

*Z*

*L C*

*L Z*

*Z*

*Z*

*R Z*

*C*

*C*

*C*

*Z*

*L C*

*Z*

*R*

*C*

_{}

_{ }

_{ }

_{}

_{}

_{} (3.19)

When the imaginary part of the FSS impedance assumes the same value as the impedance of the substrate, namely

2
1
0
*FSS* *FSS*
*d*
*FSS*
*L* *C*
*Z*
*C*
_{} _{}
(3.20)

the impedance *ZR* becomes purely real, equal to:

###

2 2 2 tan ( ) tan (k ) Re*d*

*d*

*d*

*m*

*d*

*d*

*R*

*d*

*Z*

*d*

*Z*

*R*

*R*

_{ } (3.21)

As discussed in the previous part, to achieve complete absorption of the incoming signal, the impedance in (3.21) must be equal to the free space impedance:

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

###

2 0 tan ( ) Re*d*

*d*

*d*

*d*

*R*

*opt*

*d*

*Z*

*Z*

*R*

_{ } (3.22) which yields: 2 0 tan ( )

*d*

*d*

*d*

*d*

*opt*

*d*

*R*

*Z*

_{ } (3.23)

Relation (3.23) clearly shows that the FSS resistance depends on the thickness and on the permittivity and the permeability of the medium used for the absorbing structure. It is evident that the thicker is the substrate, the higher is the optimal FSS resistance.

Ideally the optimal surface resistance of the lossy layer would be exactly equal to

*opt*

*R*

_{ if the material would be uniform. In case of a microwave absorber made with }FSS, the optimal surface resistance

*RS*has to be derived from the lumped resistance

*R* of the equivalent circuit. It depends not only on the thickness and on the
electromagnetic characteristics of the material, but also on the unit cell shape. As a
good estimate for a patch type FSS, the surface resistance can be expressed as:

2
*S*
*A*
*R* *R*
*D*
(3.24)

where *A* is the surface area of the lossy element within a single unit cell and *D* is
the cell periodicity. From (3.24) it is evident that the smaller is the scattering area,
the smaller is the surface resistance that generates the same losses with a fixed
periodicity of the cell. This expression works very well for patch type FSSs, but with
other resonant shapes, it should be considered only the surface area of the element

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

along the direction of the current with some other specific modifications related to the specific shape.

Different FSS shapes have been proposed, usually the ones we know the behavior
or we have an equivalent circuit model, such as squared patches, crosses and rings
or loops. Single-square and double-square configurations have been well studied,
*in [30] Li et al. propose the canonic single dielectric layer structure with a resistive *
treble-square loops FSS on the top (Figure 3.7). They analyze the absorber with
HFSS, obtaining three resonances at different frequencies. This result is coherent
with the equivalent circuit method, which is useful to predict the frequency
response. The lowest resonance at 11.6 GHz is mainly determined by loop 1, the
middle one at 17.9 GHz is mainly determined by both loop 1 and loop 2, and the
third one at 26.4 GHz is determined by all three loops.

**Figure 3.7 Geometry of the FSS screen proposed in [30] **

The simulations show a bandwidth, referred to -10 dB, over a frequency range of 10.7-29 GHz (Figure 3.8). Because of the symmetry of the unit cell shape, this absorber is also insensitive to the wave polarization and stable performance are obtained with different oblique incidence angles . 30

**Chapter 3- Wideband Absorbers using Frequency Selective Surfaces (FSS) **

Another example of ultra-thin absorber using a monolayer structure with a screen made by square patches FSS is presented in [31]. In this case it is mainly discussed the independence from the polarization due to the symmetric geometry of the unit cell, a very useful property in some real scenarios.

**Figure 3.8 RCS reduction with normal incidence for the absorber, using two different **

*software, proposed in [30] *

One of the difficulties of realizing a layered absorber with a metallic screen on the top is the need to have a homogenous surface resistance of the FSS cells for the whole screen. An alternative solution to the use of a metallic sheet above the absorbing layer, can be printing the frequency selective surfaces through resistive inks with a desired surface resistance. In [32] this configuration is practically realized by using a inkjet printer, making this method low-cost, simple and repeatable. In this way the surface resistance could be also ideally modified locally while printing and the thickness of the metal becomes close to zero if a high quality specific designed printer is used.